- 73 Views
- Uploaded on

Download Presentation
## PowerPoint Slideshow about ' Lecture #14' - nyssa-atkins

**An Image/Link below is provided (as is) to download presentation**
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

Presentation Transcript

Lecture #14

ANNOUNCEMENTS

- Reader with reference material from Howe & Sodini and from Rabaey et al available at Copy Central on Hearst Ave. near Euclid
OUTLINE

- Semiconductor materials
- Properties of silicon
- Doping
Reading

Howe & Sodini: Ch. 2.1-2.4.1

I

_

+

W

t

homogeneous sample

L

(Units:W)

Resistance

where r is the resistivity

Electrical Resistance(Units:W-cm)

Low resistivity => “conductor”

High resistivity => “insulator”

Intermediate resistivity => “semiconductor”

Generally, the semiconductor material used in integrated-circuit devices is crystalline

In recent years, however, non-crystalline semiconductors have become commercially very important

What is a Semiconductor?polycrystalline amorphous crystalline

Semiconductor Materials

- Elemental:
- Compound:

14 electrons occupying the 1st 3 energy levels:

1s, 2s, 2p orbitals filled by 10 electrons

3s, 3p orbitals filled by 4 electrons

To minimize the overall energy, the 3s and 3p orbitals hybridize to form 4 tetrahedral 3sp orbitals

Each has one electron and

is capable of forming a bond

with a neighboring atom

The Silicon AtomEach Si atom has 4 nearest neighbors

lattice constant

= 5.431Å

The Si Crystal“diamond cubic” lattice

Compound Semiconductors

- “zinc blende” structure
- III-V compound semiconductors: GaAs, GaP, GaN, etc.
- important for optoelectronics and high-speed ICs

Silicon is a semiconductor material.

Pure Si has relatively high resistivity at room temperature.

There are 2 types of mobile charge-carriers in Si:

Conduction electronsare negatively charged.

Holesare positively charged. They are an “absence of electrons”.

The concentration of conduction electrons & holes

in a semiconductor can be affected in several ways:

by adding special impurity atoms (dopants)

by applying an electric field

by changing the temperature

by irradiation

Electronic Properties of SiSi

Si

Si

Si

Si

Si

Si

Si

Conduction Electrons and Holes2-D representation

When an electron breaks loose and becomes a

conduction electron, a hole is also created.

Note: A hole (along with its associated positive charge) is mobile!

n = number of mobile electrons per cm3

p = number of holes per cm3

ni= intrinsic carrier concentration (#/cm3)

In a pure semiconductor,

n = p = ni

Definition of ParametersGeneration

- We have seen that conduction (mobile) electrons and holes can be created in pure (intrinsic) silicon by thermal generation.
- Thermal generation rate increases exponentially with temperature T

- Another type of generation process which can occur is optical generation
- The energy absorbed from a photon frees an electron from covalent bond
- In Si, the minimum energy required is 1.1eV, which corresponds to ~1 mm wavelength (infrared region). 1 eV = energy gained by
an electron falling through 1 V potential = qeV = 1.6 x 10-19 C x

1 V = 1.6 x 10-19 J.

- In Si, the minimum energy required is 1.1eV, which corresponds to ~1 mm wavelength (infrared region). 1 eV = energy gained by

- The energy absorbed from a photon frees an electron from covalent bond
- Note that conduction electrons and holes are continuously generated, if T > 0

Recombination

- When a conduction electron and hole meet, each one is eliminated, a process called “recombination”. The energy lost by the conduction electron (when it “falls” back into the covalent bond) can be released in two ways:
- to the semiconductor lattice (vibrations)
“thermal recombination” semiconductor is heated

- to photon emission
“optical recombination” light is emitted

- Optical recombination is negligible in Si. It is significant in compound semiconductor materials, and is the basis for light-emitting diodes and laser diodes.

- to the semiconductor lattice (vibrations)

Generation and Recombination Rates

- The generation rate is dependent on temperature T, but it is independent of n and p :
- The recombination rate is proportional to both n and p:
- In steady state, a balance exists between the generation and recombination rates.
- A special case of the steady-state condition is thermal equilibrium: no optical or electrical sources

Donors: P, As, Sb

Acceptors: B, Al, Ga, In

DopingBy substituting a Si atom with a special impurity atom (Column V

or Column III element), a conduction electron or hole is created.

Dopant concentrations typically range from 1014 cm-3 to 1020 cm-3

Charge-Carrier Concentrations

ND: ionized donor concentration (cm-3)

NA: ionized acceptor concentration (cm-3)

Charge neutrality condition: ND + p = NA + n

At thermal equilibrium, np = ni2 (“Law of Mass Action”)

Note: Carrier concentrations depend on net dopant concentration (ND - NA) !

and

N-type and P-type MaterialIf ND >> NA(so that ND – NA >> ni):

n >> p material is “n-type”

If NA >> ND(so that NA – ND >> ni):

p >> n material is “p-type”

Terminology

intrinsic semiconductor: “undoped” semiconductor

electrical properties are native to the material

extrinsic semiconductor: doped semiconductor

electrical properties are controlled by the added impurity atoms

donor: impurity atom that increases the electron concentration

group V elements (P, As)

acceptor: impurity atom that increases the hole concentration

group III elements (B, In)

n-type material: semiconductor containing more electrons than holes

p-type material: semiconductor containing more holes than electrons

majority carrier: the most abundant carrier in a semiconductor sample

minority carrier: the least abundant carrier in a semiconductor sample

3

1

electron

4

5

Carrier Scattering- Mobile electrons and atoms in the Si lattice are always in random thermal motion.
- Average velocity of thermal motion for electrons in Si:
~107 cm/s @ 300K

- Electrons make frequent “collisions” with the vibrating atoms
- “lattice scattering” or “phonon scattering”

- Other scattering mechanisms:
- deflection by ionized impurity atoms
- deflection due to Coulombic force between carriers

- Average velocity of thermal motion for electrons in Si:
- The average current in any direction is zero, if no electric field is applied.

3

1

electron

4

5

E

Carrier Drift- When an electric field (e.g., due to an externally applied voltage) is applied to a semiconductor, mobile charge-carriers will be accelerated by the electrostatic force. This force superimposes on the random motion of electrons:

- Electrons drift in the direction opposite to the E-field
Current flows

- Because of scattering, electrons in a semiconductor do not achieve constant acceleration. However, they can be viewed as classical particles moving at a constant average drift velocity.

n

p

Drift Velocity and Carrier MobilityMobile charge-carrier drift velocity is proportional to applied E-field:

| v | = mE

m is the mobility

(Units: cm2/V•s)

Note: Carrier mobility depends on total dopant concentration (ND + NA) !

+

+

Current DensityThe current density J is the current per unit area

(J = I/ A ; A is the cross-sectional area of the conductor)

If we have N positive charges per unit volume moving with average speed v in the +x direction, then the current density in the +x direction is just J = qNv

Example:

2 x1016 holes/cm3 moving to the right at 2 x104 cm/sec

J = 1.6x10-19 x2x1016 x 2x104 = 64 A/cm2

v

Suppose this occurs in a conductor 2 mm wide and 1 mm thick:

I = J x A = 64 x (2x10-4 x1x10-4)

= 1.28 mA

hole current density:

Electrical Conductivity sWhen an electric field is applied, current flows due to drift of mobile electrons and holes:

total current density:

conductivity

(Units: W-cm-1)

From mvs. ( NA + ND ) plot

ExampleConsider a Si sample doped with 1016/cm3 Boron.

What is its resistivity?

Answer:

NA = 1016/cm3 , ND= 0 (NA >> ND p-type)

p 1016/cm3 and n 104/cm3

Example (cont’d)

Consider the same Si sample, doped additionally

with 1017/cm3 Arsenic. What is its resistivity?

Answer:

NA = 1016/cm3, ND= 1017/cm3 (ND>>NA n-type)

n 9x1016/cm3 and p 1.1x103/cm3

The sample is converted to n-type material by adding more donors than acceptors, and is said to be “compensated”.

Sheet Resistance Rs

(Unit: ohms/square)

Rs is the resistance when W = L

(L, W, t = length, width, thickness)

- The Rs value for a given layer in an IC technology is used
- for design and layout of resistors
- for estimating values of parasitic resistance in a circuit

R = Rs

R = Rs/2

R = 2Rs

R = 3Rs

R 2.6Rs

Metallic contacts

Integrated-Circuit Resistors

The resistivity and thickness t are fixed for each layer in a given manufacturing process

t

A circuit designer specifies the length L and width W, to achieve a desired resistance R

fixed designable

Example: Suppose we want to design a 5 kW resistor using a layer of material with Rs = 200 W/

Space-efficient layout

Resistor layout (top view)

4 valence electrons per atom

diamond lattice: each atom has 4 nearest neighbors

5 x 1022 atoms/cm3

In a pure Si crystal, conduction electrons and holes are formed in pairs.

Holes can be considered as positively charged mobile particles which exist inside a semiconductor.

Both holes and electrons can conduct current.

Dopants in Si:

Reside on lattice sites (substituting for Si)

Group V elements contribute conduction electrons, and are called donors

Group III elements contribute holes, and are called acceptors

Summary
Download Presentation

Connecting to Server..